| ||Format||Pages||Price|| |
|4||$39.00||  ADD TO CART|
|Hardcopy (shipping and handling)||4||$39.00||  ADD TO CART|
Significance and Use
5.1 The data generated by this test method shall be used to determine whether aircraft structural aluminum alloys are liable to be corroded or damaged by application of the test material during routine maintenance operations.
5.2 Interpretation of the sandwich corrosion test results is based on a comparison of the appearance of faying surfaces of three sets of coupons. One set of test coupons is exposed with reagent water only in the faying surfaces, to establish the baseline (controls) against which the panels exposed to the test material are compared. Disregard corrosion at cut edges of the test coupons.
5.3 The relative corrosion severity rating system is provided in order to allow a numerical classification of the test results and to eliminate the necessity for elaborate weight loss measurements. Pitting corrosion, which is rated 4—extensive (severe) corrosion, may involve only a negligible weight loss.
5.4 Relative corrosion severity rating system:
0—No visible corrosion and no discoloration present
1—Very slight corrosion or very slight discoloration, and/or up to 5 % of areaA corroded
2—Discoloration and/or up to 10 % of areaA corroded
3—Discoloration and/or up to 25 % of areaA corroded
4—Discoloration and/or more than 25 % of areaA corroded, and/or pitting
1.1 This test method defines the procedure for evaluating the corrosivity of aircraft maintenance chemicals, when present between faying surfaces (sandwich) of aluminum alloys commonly used for aircraft structures. This test method is intended to be used in the qualification and approval of compounds employed in aircraft maintenance operations.
1.2 The values stated in SI units are to be regarded as the standard. The values given in parentheses are for information.
1.3 This standard may involve hazardous materials, operations, and equipment. This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use. Specific hazard statements appear in Section .
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
D1193 Specification for Reagent Water
D1748 Test Method for Rust Protection by Metal Preservatives in the Humidity Cabinet
G46 Guide for Examination and Evaluation of Pitting Corrosion
ICS Number Code 49.025.99 (Other materials)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM F1110-09(2014), Standard Test Method for Sandwich Corrosion Test, ASTM International, West Conshohocken, PA, 2014, www.astm.orgBack to Top